HAL Id: tel-01789430
https://tel.archives-ouvertes.fr/tel-01789430Submitted on 10 May 2018
HAL is a multi-disciplinary open access archive for the deposit and dissemination of sci-entific research documents, whether they are pub-lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.
Luis Alfredo Rodríguez González
To cite this version:
Luis Alfredo Rodríguez González. In situ Lorentz microscopy and electron holography in magnetic nanostructures. Materials Science [cond-mat.mtrl-sci]. Université Toulouse III Paul Sabatier (UT3 Paul Sabatier); Universidad de Zaragoza, 2014. English. �NNT : 2014TOU30228�. �tel-01789430�
%COLE 5NITÏ $IRECTEURS 2APPORTEURS LE MEMBRES
Université Toulouse III Paul Sabatier (UT3 Paul Sabatier)
Sciences de la Matière (SDM)
IN SITU LORENTZ MICROSCOPY AND ELECTRON HOLOGRAPHY
IN MAGNETIC NANOSTRUCTURES
mercredi 17 décembre 2014
Luis Alfredo Rodríguez González
Dr. Agustina Asenjo Barahona, Científico Titular au CSIC (Espagne)
Dr. Francisco Rivadulla Fernández, Professeur à l'Universidad de Santiago de Compostela -(Espagne)
Dr. Etienne Snoeck, Directeur de Recherche au CNRS-CEMES (France) Dr. César Magén Dominguez, Researcher ARAID, INA-UNIZAR (Espagne) Centre d'Élaboration de Matériaux et d'Études Structurales (CEMES-CNRS)
Dr. Jose Maria de Teresa, Profesor de Investigación au CSIC (Espagne) Dr. Michel Goiran, Professeur à l'Université Paul Sabatier - LNCMI-CNRS (France) Dr. Christophe Gatel, Maitre de Conférence à l'Université Paul Sabatier, Membre Junior de
Laboratorio de Microscopías Avanzadas (LMA) Instituto de Nanociencia de Aragón (INA) Universidad de Zaragoza
Structurales - Centre Nationale de la Recherche Scientifique (CEMES-CNRS) Université Paul Sabatier
In situ Lorentz Microscopy and Electron
Holography in Magnetic Nanostructures
Luis Alfredo Rodríguez González
Zaragoza, November 2014
César Magén Dominguez
Dedicado a Dios, mis Padres y Hermanos, y a mi esposa Lorena Marín
In this Thesis, we have developed quantitative and qualitative studies of the magnetic states of different ferromagnetic nanostructures by in situ Lorentz Microscopy (LM) and Electron Holography (EH) experiments under the application of magnetic fields or at low temperature (100 K). A detailed investigation was performed in three different ferromagnetic nanostructures: L-shape cobalt and Co50Fe50 nanowires grown
by Focused Electron Beam Induced Deposition (FEBID) and Electron Beam Lithography (EBL) techniques, respectively; square cobalt antidot arrays fabricated by the combination of sputtering and Focused Ion Beam (FIB) techniques; and epitaxially strained La2/3Ca1/3MnO3 (LCMO) thin films grown by Pulsed Laser Deposition (PLD).
In addition, the traditional method to perform in situ LM and EH experiments with the application of controlled magnetic fields through the objective lens has been optimized. We have built the mathematical description that permits the total control of the in-plane component of the magnetic field produced by the objective lens. Such in-plane magnetic field was widely employed to perform magnetization reversal studies in the magnetic nanowires and antidot arrays.
In the ferromagnetic nanowires, we have realized a quantitative study of the reversal magnetization process through the manipulation of single domain walls (DWs). In the case of the L-shape Co nanowires, the DW nucleation process has been correlated with the lateral dimensions and thickness of the nanostructure. For a particular series of 500-nm-wide cobalt nanowires, we detected a progressive variation of the magnetic configuration of the nucleated DW with the increase of the thickness. These configurational changes produced important effects in the thickness dependence of the nucleation field (HC), such as a maximum value just in the crossover between an
asymmetry transversal wall and asymmetry vortex wall. In the case of the notched L-shape Co50Fe50 nanowires, in situ LM experiments allowed evaluating the
pinning/depinning quality of a single DW by an increasing magnetic field. For such evaluation, series of notches arranged along one branch of the L-shape nanowire were
fabricated. We found that a series of curved notches presented the best pinning/depinning behavior.
In the cobalt antidots arrays (holes of 55 nm diameter), the remanent magnetic states for different antidot periodicities (p) were explored. For the magnetic analysis of antidot arrays with small periodicities (p 160 nm), a low-frequency filtered method was implemented to enhance the magnetic contrasts observed inside the array through Fresnel-mode LM. In antidot arrays with 116 p 160 nm, we found that the magnetic structure is mainly composed by extended superdomains and unit-cell-wide confined superdomains called magnetic chains. Magnetization reversal LM experiments in an antidot array with p = 160 nm showed that the magnetization switching occurs by the nucleation and propagation of superdomain walls (SDWs), and a clear differences were observed as a function of the magnetic field orientation: while the magnetization switching by the application of magnetic fields transversal to the antidot rows occurs by the simultaneous nucleation and propagation of horizontal and vertical (SDWs), the switching process under magnetic fields parallel to the horizontal antidot rows takes place in two stages: the system first nucleates and propagates horizontal SDWs, and then nucleates and propagates vertical SDWs.
Finally, we achieved the direct visualization of the magnetic configuration of strained LCMO thin films at 100 K using a cryogenic TEM holder, which allowed observing the effects of the substrate-induced strain on the magnetic properties of the films. While LCMO thin films grown on an SrTiO3 substrate (tensile induced strain)
present a magnetic phase separation effect with a non ferromagnetic layer at the surface of the film, LCMO thin films grown on LaAlO3 (compressive strain) present an
out-of-plane magnetocrystalline anisotropy. These anomalous behaviors were contrasted with macroscopic magnetic measurements finding that they account for an apparent reduction of the saturation magnetization. The evidence of an exchange bias effect and theoretical calculation allowed concluding that the non-ferromagnetic layer has an antiferromagnetic ordering.
En esta Tesis, hemos desarrollado estudios cualitativos y cuantitativos de los estados magnéticos de diferentes nanoestructuras ferromagnéticas mediante experimentos in situ de Microscopia Lorentz (LM) y Holografia Electrónica (EH) con la aplicación de campos magnéticos o trabajando a bajas temperaturas (100 K). Se ha realizado una investigación detallada en tres diferentes nanoestructuras ferromagnéticas: (1) nanohilos de Cobalto y Co50Fe50 en forma de “L”, crecidos
respectivamente por técnicas de deposición inducida por haz de electrones focalizados (FEBID) y litografía por haz de electrones (EBL); (2) redes cuadradas de antidots de cobalto fabricadas combinando técnicas de sputtering y litografía por haz de iones focalizado (FIB); y (3) láminas delgadas epitaxiales de La2/3Ca1/3MnO3 (LCMO)
crecidas por la técnica de deposición por laser pulsado (PLD). Además se ha optimizado el método tradicional para realizar experimentos in situ de LM y EH con la aplicación de campos magnéticos a través de la lente objetivo. En esta optimización, hemos elaborado una descripción matemática que permite el control total de la componente en el plano de la muestra del campo magnético producido por la lente objetivo. Esta componente en el plano se ha usado ampliamente para desarrollar los diferentes estudios de la inversión de la imanación en los hilos y matrices de antidots ferromagnéticos que se presentan a continuación.
En el caso de los nanohilos magnéticos, se ha realizado un estudio cuantitativo de los procesos de inversión de la imanación a través de la manipulación de paredes de dominio (DW) individuales. En el caso de nanohilos de Co en forma de “L”, se han estudiado los procesos de nucleación de DW en función de las dimensiones laterales de la nanoestructura y de su espesor. Para una serie particular de nanohilos de Co de 500 nm de anchura, se detectó una variación progresiva de la configuración magnética de las DW nucleadas al aumentar el espesor. Estos cambios de configuración produjeron efectos importantes en la dependencia del campo coercitivo (HC) con el espesor tales
asimétrica y una pared tipo vórtice asimétrica. En el caso de los nanohilos de Co50Fe50
con nanoconstricciones también con forma de L, experimentos in situ de LM han permitido evaluar la calidad del anclaje/desanclaje de DW individuales al incrementar el campo magnético. Para esta evaluación, se fabricaron series de nanoconstricciones dispuestas a lo largo de uno de los brazos del nanohilo, donde se ha analizado cuál es la serie de muescas que presenta un mejor comportamiento de anclaje/desanclaje.
También se han estudiado los estados magnéticos remanentes de redes antidots de cobalto con agujeros de 55 nm de diámetro y diferentes periodicidades (p). Para la exploración de las propiedades magnéticas de redes de antidots con periodicidades bajas (p 160 nm), se ha implementado un método de filtrado a bajas frecuencias para aumentar los contrastes magnéticos observado dentro de las redes a través de LM en modo Fresnel. En redes de antidots con 116 p 160 nm, se encontró que la estructura magnética se compone principalmente de superdominios magnéticos y cadenas magnéticas con una anchura de una celda unidad. Experimentos de inversión de la imanación a través de LM en el arreglo de antidots de 160 nm de periodicidad han demostrado que tal inversión ocurre por la nucleación y propagación de paredes de superdominio magnéticas (SDWs), y se ha observado una clara diferencia en función de la orientación del campo magnético aplicado: mientras ésta ocurre por la nucleación y propagación simultanea de SDWs cuando se aplica campos magnéticos transversales a las columnas de antidots, campos magnéticos paralelos a las columnas de antidots producen un inversión de la imanación en dos etapas: el sistema primero nuclea y propaga SDWs horizontales, para luego nuclear y propagar SDWs verticales.
Finalmente, la visualización directa de la configuración magnética de láminas delgadas tensionadas de LCMO a baja temperatura nos ha permitido analizar los efectos de la tensión epitaxial inducida por el sustrato en las propiedades magnéticas de las láminas. Mientras las láminas crecidas sobre sustratos de SrTiO3 (tensión expansiva)
presentan un efecto de segregación de fase magnética donde una capa no ferromagnética se forma en la superficie de la manganita, láminas de LCMO crecidas sobre sustratos de LaAlO3 (tensión compresiva) exhiben una anisotropía magnetocristalina fuera del
plano del sustrato. Estos comportamientos anómalos se han contrastado con medidas macroscópicas de imanación encontrando que dan buena cuenta de la aparente reducción de la imanación de saturación y de la forma de los ciclos de histéresis. Medidas adicionales en las que se ha observado el fenómeno de exchange bias, así como cálculos teóricos han permitido concluir que la capa superficial no ferromagnética tiene un ordenamiento antiferromagnético.
L'objectif général de la thèse vise à développer des mesures quantitatives des configurations magnétiques locales dans des matériaux nanostructurés par des études in-situ en microscopie de Lorentz (LM) et holographie électronique (EH) sous l’application de champs magnétiques extérieurs et à basse température (100 K). Ce travail fait partie d’une collaboration entre les deux groupes de recherche du LMA -INA et du CEMES–CNRS.
Dans la première partie de ma thèse, je me suis attaché au développement d’une procédure d’expérience in-situ en LM et EH permettant de contrôler le champ magnétique appliqué dans le plan de l’objet étudié en utilisant le champ magnétique produit par la lentille objectif. Ceci est réalisé en adaptant l’excitation de la lentille objectif et en ajustant l’orientation de l’objet plongé dans ce champ pour contrôler l’intensité et la direction du champ appliqué. J’ai évalué les performances et les limitations de cette procédure d’application d’un champ in-situ en MET au travers de deux études : 1/ le contrôle de la position des parois de domaine magnétiques (DW) dans un nano-anneau de Co déposé par FEBID, 2/ l’étude de l'effet de la composante magnétique hors-plan sur la mesure du champ coercitif des films minces monocristallins de manganite et d’un nanofil polycristallin de Co.
Dans une deuxième partie, j’ai utilisé cette méthode de pour étudier les processus de nucléation et propagation de DWs dans les nanofils de Co en forme de « L ». Nous avons étudié les configurations de DWs et leurs champs de nucléation et de propagation pour différentes épaisseurs de nanofils. Pour une largeur donnée de nanofils (500 nm), nous avons trouvé que pour des épaisseurs t < 13 nm le DW est une paroi transverse alors que pour des épaisseurs t > 13 nm elle est de configuration vortex. En outre, c’est à cette transition que la paroi est la plus mobile et que la différence entre les champs de nucléation et propagation est la plus grande offrant la possibilité de manipuler facilement cette paroi et d’envisager des applications dans le domaine de l’enregistrement magnétique. J’ai également étudié localement in-situ les processus de
piégeage/dé-piégeage de DWs dans des nanofils de Co50Fe50 sur lesquels ont été gravé
des nanoconstrictions de diverses formes.
Dans une troisième partie, nous avons étudié les configurations magnétiques dans des réseaux d’antidots ferromagnétiques fabriqués à partir d’une couche mince de cobalt. Nous avons tout d’abord étudié l’effet de la géométrie du système (périodicité des réseaux, tailles des trous) sur les configurations magnétiques à rémanence. Pour périodicités p ≤ 160 nm, nous avons observé la formation de « superdomaines » magnétiques. Pour améliorer la visualisation de ces superdomaines par LM, j’ai développé une méthode de filtrage de Fourier de basse fréquence. J’ai ensuite mené des études in-situ en LM en effectuant des cycles d'hystérésis avec un champ appliqué parallèlement aux rangées d’antidots puis dans la diagonale des réseaux. Nous avons mis en évidence des modes de propagation de DWs et des mécanismes de renversement d’aimantation distincts.
La quatrième partie de ma thèse est consacrée au développement d’études LM et EH in-situ à basse température pour étudier les effets de contraintes épitaxiales sur les propriétés magnétiques de couches minces épitaxiales de manganites : La2/3Ca1/3MnO3
(LCMO). Nos études à basse température sur diverses couches de LCMO épitaxiées sur différents substrats (SrTiO3, LaSr,AlTaO3 and LaAlO3) ont permis pour la première fois
une caractérisation directe de l'aimantation locale dans les couches minces épitaxiées de LCMO. Nous avons mis en évidence la formation d’une couche non ferromagnétique à la surface du film mince de LCMO dépendant de l’état de contrainte (en compression) de la couche; la variation de l'anisotropie magnétocristalline variant avec la contrainte épitaxiale lorsque le film est en tension; la disparition de la couche non ferromagnétique lorsque que la couche de LCMO contrainte relaxe par traitement thermique. Tous ces résultats expérimentaux ont été confortés par des mesures macroscopiques complémentaires que nous avons menées par magnetometry SQUID et par des simulations théoriques prenant en compte les effets de contraintes sur les propriétés magnétiques dans ces couches d’oxydes
1 Introduction ... 1
1.1 Magnetism: a brief history and its importance ... 1
1.2 Fundaments of Magnetism ... 3
1.2.1 Quantum origin of magnetic order ... 3
1.2.2 Fundaments of ferromagnetism ... 6
1.2.3 Micromagnetic energy ... 7
1.2.4 Micromagnetic simulation ... 11
1.3 Objectives and outline of the Thesis ... 12
1.4 References ... 15
2 Experimental Techniques ... 17
2.1 TEM magnetic imaging ... 17
2.1.1 Introduction ... 17
2.1.2 Image formation in TEM ... 20
2.1.3 Electron beam phase shift measurements: recording the magnetism ... 25
2.1.4 The objective lens ... 26
2.2 Lorentz microscopy ... 30
2.2.1 Transport of Intensity Equation (TIE) ... 33
2.2.2 Phase reconstruction and magnetic induction mapping by Lorentz microscopy ... 35
2.3 Off axis electron holography ... 37
2.3.1 Phase reconstruction in electron holography ... 40
2.3.2 Phase shift separation and interpretation of the magnetic contribution ... 41
2.4 Remarkable aspects of Lorenz microscopy and electron holography ... 45
2.5 DualBeam ... 47
2.5.1 Introduction ... 47
2.5.2 Focused electron beam induced deposition (FEBID) ... 48
2.5.3 Focused ion beam (FIB) ... 50
184.108.40.206 FIB milling: lithography patterning... 51
220.127.116.11 FIB milling: TEM sample preparation ... 52
2.6 Image-corrected FEI Titan3 60-300 ... 53
References ... 55
3 In situ TEM characterization of magnetic nanostructures under external magnetic field ... 63
3.1 Motivation ... 64
3.2 Magnetic field calibration ... 66
3.3 Calibration of the in-plane component of the OL magnetic field .... 67
3.4 Influence of the out-of-plane magnetic field component in the in situ experiment ... 73
3.5 Quantitative hysteresis loops in nanostructures with high shape anisotropy ... 76
3.6 Conclusions ... 84
References ... 86
4 Domain wall manipulation in Co and notched Co50Fe50 nanowires ... 91
4.1 Motivation ... 91
4.2 Experimental details ... 93
4.3 Optimized cobalt nanowires grown by FEBID for domain wall manipulation ... 95
4.3.1 Lateral size and thickness dependence of the DW nucleation ... 95
4.3.2 Magnetic configuration of domain wall in 500-nm-wide FEBID cobalt nanowires ... 101
4.4 Field-driven domain wall manipulation in Co50Fe50 nanowires
with nanoconstrictions ... 105
4.4.1 Domain wall nucleation and depinning process in the corner of L-shaped Co50Fe50 nanowires ... 105
4.4.2 Domain wall transmission through the nanoconstrictions ... 110
4.5 Conclusions ... 112
References ... 114
5 High-resolution imaging of remanent states and magnetization reversal processes in high density cobalt antidot arrays ... 119
5.1 Motivation ... 119
5.2 Experimental details ... 121
5.3 Microstructural characterization of the antidot arrays ... 122
5.4 Magnetic imaging at remanence ... 127
5.4.1 A qualitative description: defocused Lorentz microscopy images ... 127
5.4.2 A quantitative description: TIE reconstruction procedures .. 132
5.5 Magnetization reversal processes... 138
5.6 Fresnel contrast formation of superdomain walls ... 145
5.7 Conclusions ... 150
References ... 152
6 Strain-induced effects on the magnetic properties of epitaxial La2/3Ca1/3MnO3 thin films ... 157
6.1 Motivation ... 157
6.2 Experimental details ... 160
6.3 Structural properties of LCMO thin films ... 162
6.4 Strain effect dependence of the magnetic properties of LCMO thin films ... 169
6.5 Direct visualization of the remanent state of LCMO thin films ... 175
6.7 Conclusions ... 187
References ... 189
7 Conclusions and outlooks... 197
List of publications ... 205
2VW: Double Vortex Wall. AFM: Antiferromagnetic.
ATW: Asymmetric Transversal Wall. AVW: Asymmetric Vortex Wall. C-FEG: Cold Field Emission Gun. CNW: Curved Notch Wire. CTEM: Conventional TEM. DFT: Density Functional Theory. DPC: Differential Phase Contrast. DW: Domain Wall.
EA: Easy Axis.
EBL: Electron Beam Lithography. EELS: Electron Energy Loss
EH: Electron Holography. FC: Field Cooling.
FEBID: Focused Electron Beam Induced
FFT: Fast Fourier Transform.
FFT-1: Inverse Fast Fourier Transform.
FIB: Focused Ion Beam.
FIBID: Focused Ion Beam Induced
GGA-PBE: Generalized Gradient
Approximation – Perdew-Burke-Ernzerhof. GIS: Gas-Injection-System. GMR/TMR: Giant magnetoresistance/Tunnel magnetoresistance.
GPA: Geometry Phase Analysis. GPU: Graphical Processor Unit. HA: Hard Axis.
HAADF: High Angle Annular Dark Field. HRTEM: High Resolution Transmission
LE-SDW: Low-Energy Superdomain
LF: Lorentz Force.
LLG: Landau-Lifshitz-Gilbert. LM: Lorentz Microscopy. LMIS: Liquid-Metal Ion Source. LSMO: La2/3Sr1/3MnO3.
MBE: Molecular Beam Epitaxy. MC: Magnetic Chain.
MFM: Magnetic Force Microscopy. MOKE: Magneto-Optical Kerr Effect. MRAM: Magnetoresistive
MTJ: Magnetic Tunnel Junction. M-XTM: Magnetic X-ray Transmission
NW: Nanowire. OL: Objective lens. OOMMF: Object Oriented
RNW: Rectangular Notch Wire. SD: Superdomain.
SDW: Superdomain Wall.
SEM: Scanning Electron Microscopy. SEMPA: Scanning Electron Microscopy
with Polarization Analysis.
S-FEG: Schottky Field Emission Gun. SIMS: Secondary Ion Mass Spectroscopy. SPLEEM: Spin-Polarized Low-Energy
SP-STM: Spin-Polarized Scanning
SQUID: Superconducting Quantum
STEM: Scanning Transmission Electron
STXM: Scanning Transmission X-ray
TEM: Transmission Electron
TIE: Transport of Intensity Equation. TNW: Triangular Notch Wire. TW: Transversal Wall. VW: Vortex Wall.
XEDS: X-ray Energy-Dispersive
XFEG: High brightness Field Emission
XMCD-PEEM: X-ray Magnetic Circular
Dichroism – PhotoElectron Emission Microscopy.
XRD: X-Ray Diffraction. ZFC: Zero Field Cooling.
1.1. Magnetism: a brief history and its importance
Just take a glance around us to realize that Magnetism plays a crucial role in our modern life. Most of the technological devices of daily use are based on or contain magnetic materials: TVs, cell phones, computer hard disks, credit cards, speakers, electric motors, sensors… the list would be never-ending. More than 2500 years have passed since the man discovered the first magnetic material, the magnetite (Fe3O4), and
the human wasted no time in exploiting its attractive properties.
Historically, the first practical application of Magnetism was documented in China, between 221-206 BC, with the invention of the “south pointer”. This ancestor of the compass was a lodestone carved with a spoon shape that rotated on a surface to align its handle, magically, with the Earth’s magnetic field. Considered of divine nature, the south pointer was initially a tool to predict the fortunate location for burials sites, harmonic building construction and even decision-making in Chinese culture (nowadays it is used as part of feng shui), but then hunters began to use it as a tool that prevented them from getting lost in their journeys. More than 14 centuries passed before the Chinese started to fabricate compasses for navigation purpose for military orienteering (1040-1044 AC) and maritime navigation (1111-1117 AC).
At the beginning of the 17th century, William Gilbert wrote in his book “De Magnete” the first truly scientific study of Magnetism known to that date, giving explanation of some magnetic phenomena formerly attributed to superstition. He investigated the properties of iron magnets and lodestones, and formed a clear picture of the Earth’s
magnetic field. In 1743, Daniel Bernoulli invented one of the most iconic symbols of Magnetism: the horseshoe magnet. The idea arose as an attempt to solve the problem of building a reasonably compact magnet that did not destroy itself in its own demagnetizing field. The greatest advances in the understanding of the magnetic phenomenology were achieved in the 19th century. The works of Hans Christian Ørsted, André-Marie Ampère and Dominique François Jean Arago in 1820 demonstrated the relationship between electricity and magnetism, while Michael Faraday discovered in 1845 the connection between magnetism and light (magneto-optic Faraday effect). These discoveries inspired them to develop the key principles of future technologies as revolutionary as the electromagnetic telegram (proposed by Ampère) and an electric motor (proposed by Faraday). All these experimental works, together with other works in the field of electricity, inspired James Clerk Maxwell to formulate a unified theory of electricity, magnetism and light in 1864, which was subsequently summarized in the four famous equations known as the Maxwell’s equations. The Revolution of the Magnetism started! This boosted a fast development of electromagnetic energy converters (motors and generators), electromagnetic propagation devices (radios, televisions, antennas, radars), and helped to develop new groundbreaking theories… such as the Theory of the Relativity . The 20th century progresses on Magnetism were
focused on the understanding of its microscopic origin. In 1907 Pierre Weiss gave a successful explanation of the loss of ferromagnetism above the Curie point through the molecular field theory. He also theorized that magnetic materials were composed by numerous microscopic magnets (“domains”), randomly oriented in a virgin ferromagnet that were reoriented along the external field when the system was magnetized. Later on, the discovery of the spin of the electron by George Uhlenbeck and Samuel Goudsmit in 1925 paved the way to Werner Heisenberg, who postulated in 1929 the quantum-mechanical origin of ferromagnetism through a Hamiltonian that represents the exchange interaction between two neighboring atomic spins. The advances in the understanding of Magnetism at the atomic scale allowed the development of important methods such as the magnetic resonance (in the 1940s and 1950s) and the introduction of powerful spectroscopic and diffraction techniques that permitted the determination of the magnetic and electronic structure of solids. In addition to traditional
electromagnetic and electromechanical devices, ferromagnets were used in the second half of the 20th century as data storage media. From credit cards to magnetic recording
tapes and hard disk drives, the multidomain nature of magnetic materials is still currently exploited to satisfy the demand for ever-increasing data storage density, currently approaching 1 Tbit/inch2 . Nowadays, new trends on applied Magnetism
aim at manipulating the spin transport electronics (Spintronics) in order to improve the performance of devices purely based on charge transport. This includes devices to read, write and store data, such as Giant Magnetoresistance (GMR) and Tunnel Magnetoresistance (TMR) read heads, magnetoresistive random-access memories (MRAMs) and racetrack memories, but also magnetic sensors and magnetic logic circuits . In the last decade novel, even more ambitious and unexpected applications of Spintronics have been envisaged as a potential alternative to semiconductor electronics based on spin-only transport due to Rashba-type spin-orbit coupling [4,5], or in energy harvesting based on the use of temperature gradients to produce spin currents in the so-called spin-Seebeck effect .
1.2. Fundaments of Magnetism 1.2.1. Quantum origin of magnetic order
The magnetism has its origin in the magnetic moment of the atoms produced by the angular momenta of its constituent electrons. Each atomic electron presents two types of angular momenta: an orbital moment, L, associated to the orbital motion of the electron around the nucleus, and a spin momentum, S, which is intrinsic to its nature, see Figure 1.1. Most of the atoms are composed by several electrons, and their individual orbital angular moments couple to produce a total orbital angular momentum of L = ili. The same occurs with the spin angular moment, so S = isi. Thus, the
electronic magnetic moment, , associated to each total atomic angular momenta can be expressed as:
B (Eq. 1.1)
B (Eq. 1.2)
where B is the Bohr magneton, a physical constant depending on the electron charge,
e, electron rest mass, m, and reduced Planck constant, ħ, [B = eħ/(2m) = 9.27410-24
Figure 1.1. Sketch representative of the two angular momenta associated to the electron: orbital (L) and spin (S) angular momentum. Green and yellow balls ideally represent the electron and nucleus respectively.
Thus, the total magnetic moment in the atom is then given by
According to the Pauli exclusion principle  and the Hund’s rules , atoms with “closed electronic shells” (their orbitals fully occupied) have a net magnetic moment equal to zero because, in each shell, the electrons are paired: there are as many electrons orbiting or spinning in one direction as in the opposite direction, so the net magnetic moment in each shell is zero. Atoms with “partially filled electronic shells” have however unpaired electrons, usually in the outermost shell, that contribute to produce a net atomic magnetic moment different to zero. Thus, unpaired electrons in the atomic
shells produce the magnetic response of the materials. This atomic magnetic moment will be equal to
B (Eq. 1.4)
where J is the total electronic angular momentum of the unpaired electrons and gJ is
called the Landé g-factor, which is related with the different total quantum numbers L, S, and J
gJ (Eq. 1.5)
Even if Equation 1.4 considers both orbital and spin angular momenta of the atom, the largest contribution to the total magnetic moment is due to the spin, which is 10 times stronger that the orbital angular momentum, for instance, in the ferromagnetic elements Fe, Co and Ni . In an arrangement of atoms (e.g., a crystal lattice), the atomic magnetic moments of neighboring atoms interact with each other through a quantum phenomenon known as exchange interaction. Proposed for first time by Heisenberg in 1928 , two atoms with unpaired electrons of spins Si and Sj interact
with an energy j i ij J S S 2
where Jij is the exchange constant. If Jij > 0, the energy is lowest when Si is parallel to
Sj, while Jij < 0, an antiparallel alignment of the spins will minimize the energy. Thus,
the type of exchange interaction defines the type of magnetism: in absence of an external magnetic field, a parallel alignment of spins produces a long-range ferromagnetic (FM) order, while an antiparallel alignment of neighboring spins induces an antiferromagnetic (AFM) order.
1.2.2. Fundaments of ferromagnetism
Ferromagnetism is a term used to refer to a material with a strongly magnetic behavior like permanent magnets. Historically, these ferromagnetic materials were the first magnetic materials discovered and, for this reason, the term “magnetic materials” has been traditionally assigned to them. From a macroscopic point of view, a microscopic ferromagnetic order induces a spontaneous magnetization at zero applied magnetic field, where the magnetization (M) is defined as the magnetic moment density per volume unit. The existence of a net magnetization produces around the material a magnetic induction field, which results in the strong attractive or repulsive force that magnetic materials exert on other ferrous materials. The first theory explaining such spontaneous magnetization was postulated by P. Weiss in 1907 . He considered that, in the site of each spin, there is an effective field produced by the interaction with the neighboring spins. Thus, effective induction field, B, that one spins feels is
W (Eq. 1.7)
where M is the total magnetization of the system and W is the mean field parameter
that represents the strength of the interaction (Weiss constant). These ordered spin states could be altered by the temperature. When the temperature of the system increases, the thermal agitation introduced in the ensemble destroys such long-range spin order. Above a critical temperature, called Curie temperature (TC), the thermal excitation
dominates and their magnetic moments are randomly oriented, producing a paramagnetic state. Thus, Curie temperature and spontaneous magnetization are two characteristic parameters of ferromagnetic materials.
Another important feature of ferromagnetic materials is the fact that, even if the exchange interaction is strong enough to align all spins in the same direction at microscopic scale, this state cannot be preserved macroscopically unless an external magnetic field is applied. In a micromagnetic scale, not only the exchange interaction and thermal excitation contributes to the internal energy of the system, there are other
energy contributions related to additional factors such as the crystal structure, the shape, the external magnetic field, stress and magnetostriction.
1.2.3. Micromagnetic energy
The equilibrium state of a ferromagnetic material is determined by the minimization of the total “magnetic” Gibbs free energy of the system. This is composed by the sum of several energy contributions
ms stress Z d a ex tot
where the first three terms are intrinsic to the ferromagnetic material: exchange (ex),
magnetocrystalline anisotropy (a) and demagnetizing (d) energies. The fourth energy
is associated to the response of the material to the application of an external magnetic field, the Zeeman energy (Z). The last two energy terms are related to applied stress
and magnetostriction, and their contribution to the total energy is very small, so that they are usually neglected. More in detail, each energy contribution acts in the system as follow:
Exchange energy: It is caused by the exchange coupling between the spins to tend to line them up in the same direction. The exchange energy can be expressed as an integral overall volume, V,
dV M A S ex 2 M
where is the gradient operator applied to the magnetization vector and A is the exchange constant. This energy tends to favor that the spins are always parallel between them. The Heisenberg model used to deduce Equation 1.9 describes suitably the direct exchange interaction between two ions; other models such superexchange [12,13] (in oxides) or
Ruderman-Kittel-Kasuya-Yoshida (RKKY) [14–16] (in metals) are used to describe indirect exchange interactions.
Magnetocrystalline energy: This energy contribution reflects the interaction of the magnetization with the crystal lattice. It is associated to the Coulomb interaction between the electrons of a magnetic ion and the surrounding ions in a crystal. The coordination and symmetry of the crystal environment affect the spatial distribution and population of the orbitals of the magnetic ions and, through the spin-orbit coupling, this causes a preferred orientation of the magnetization with respect to the crystal. Thus, this magnetization easy axis depends on the crystal structure of the magnetic material. In the case of uniaxial anisotropy (only one preferential magnetization direction), the first term of the magnetocrystalline anisotropy is
K dV aUni sin ( ) 2
where is the angle between the easy axis and the magnetization, and K the anisotropy constant. However, in cubic crystals (with more than one preferential magnetization direction allowed by symmetry)
(12 22 22 32 12 32 1 0
VaCub (Eq. 1.11)
where K0 and K1 are anisotropy constants and the s (s = 1, 2 and 3) are direction
cosines, i.e., the cosines of the angle between the magnetization and the crystal axis.
Demagnetizing energy (or magnetostic energy): The demagnetizing energy is also an anisotropy term related to the geometry of the nanostructure (also called shape anisotropy). It could be expressed as
dV d d
MH 2 1
where Hd is the demagnetizing field, which depends on the magnetic
configuration of the system, which in turn depends on the shape of the magnetic material. If the magnetization of the specimen is oriented in one direction (for instance, by means a strong magnetic field), “magnetic free poles” appear producing a magnetic field directed opposite to the magnetization. Its intensity is proportional to the magnetic free pole density and the shape of the specimen
NM Hd 0 1
where 0 is the magnetic permeability, M is the magnitude of the magnetization
and N is the demagnetizing factor, which depends only on the shape of the specimen. The demagnetizing or stray field has important implications in ferromagnetic materials: it is the magnetic field produced by permanent magnet and, at the same time, induces the formation of “magnetic domains”.
Zeeman energy: This is the energy contribution of a magnetic material embedded in an external magnetic field, H. Similar to the demagnetization energy, Zeeman energy is expressed as
The Zeeman energy favors the alignment of the spins parallel to the external magnetic field. If it is very strong, the total energy of the system is minimized by reaching its maximum magnetization, which is the same magnetization of each magnetic domain. In this condition, a ferromagnetic system is saturated.
Thus, the final stationary micromagnetic state of a magnetic body minimizes the total magnetic energy of the system, i.e., the sum of the different energy terms of the equation 1.8. If we consider an equilibrium state free of external magnetic fields (Z =
0), with a temperature sufficiently low that the thermal energy can be neglected (i.e., T<< TC), a saturation magnetization condition along the easy magnetization direction
will minimize both exchange and magnetocrystalline energies. However, this configuration will induce the appearance of positive and negative magnetic charges at the surfaces, producing a large demagnetizing field. To decrease the demagnetizing energy, the local magnetization close to the magnetic charges tends to rotate, orientating parallel to the surface edge. This effect favors the minimization of the d by the reduction
of the stray field, but disfavors ex and/or a. The best solution found by the system is to
break into small regions where the magnitude of the magnetization is the same in each point, but their direction is different with respect to the neighboring regions. Thus the competition of the different terms of micromagnetic energy produces magnetic domains in a ferromagnetic material, see Figure 1.2. The shape and size of each domain, as well as the magnetic configuration of all magnetic domains in ferromagnets, depend on the precise balance between these terms, which is determined by the magnetic parameters of the material (exchange constant, A; anisotropy constant, K, saturation magnetization, MS), the shape of the structure (demagnetizing factor, N) and the magnetic history.
Figure 1.2. Formation of magnetic domains: (a) alignment of the magnetization results in an intensive stray field (large magnetostatic energy); (b) division into small magnetic domains permits the reduction of the magnetostatic energy. Image extracted to Ref. .
1.2.4. Micromagnetic Simulation
Magnetic states in a ferromagnetic can be perfectly simulated by the Landau-Lifshitz-Gilbert (LLG) equation [17,18], which defines the time evolution of the magnetization under a local effective magnetic field Heff. Such magnetization equation
of motion is usually expressed as
) ( eff S eff M dt d H M M H M M
where Heff, and are the effective field, gyromagnetic ratio and damping parameter,
respectively. According to Brown´s theory , the effective field can be expressed as a functional derivative of the average energy density, E, as a function of the magnetization: M H tot eff E 0 1
where tot = V (Etot) dV. This means that Etot will correspond to the sum of the all
integrands of Equations 1.9, 1.10, 1.11, 1.12 and 1.14. This effective field exerts a torque on the magnetization vector of each “magnetic unit cell” that induces a precession movement, which is described by the first term of Equation 1.15. The magnetization is reoriented toward the effective field following a damping process as a function of time, which is described by the second term of Equation 1.15. There are very few situations where the LLG equation can be solved analytically; in general we need to use numerical methods for its solution. In addition, Equation 1.15 is only valid assuming that: (i) magnetization is a continuous function of the position, M = M(r); (ii) magnetization modulus is constant in every point and equal to the saturation magnetization, |M| = MS.
There are several micromagnetic simulation packages available to solve the LLG equation such as Nmag , Mumax3 , MicroMagnum  and OOMMF  among others, being the last one the most commonly used. However, all micromagnetic
simulations of this Thesis have been carried using the GPMagnet software package . This software performs highly efficient micromagnetic simulations thanks to the use of standard code running in a Graphical Processor Unit (GPU), taking advantage of its potential to make parallel calculations. For instance, in comparison with classical OOMMF package, the computational time of GPMagnet is reduced by two orders of magnitude. The aim of the simulation is to minimize the total energy of the magnetic system, which is usually subdivided in a rectangular mesh of prisms, called magnetic unit cell, with lateral sizes preferably less than the characteristic exchange length, lex =
(2A/0MS2)1/2, of each magnetic material (in most ferromagnets lex has a value of 2-6 nm
). The simulation starts from an initial magnetization state that can be stimulated with an external magnetic field. Generally, such initial magnetization conditions does not represent the magnetic state with minimum energy, so the simulation runs iteratively to minimize the energy until a given convergence criteria is satisfied, which could be either a maximum numbers of iterations or that the variation of the magnetization of the system with the time reaches a certain minimum value. The final magnetic configuration is considered the equilibrium state for a given external magnetic field. The solution of the Equation 1.15 allows calculating the magnetization direction distribution through the dynamic evolution of the system. However, if we are only interested in determining the magnetization distribution at equilibrium (static method), it is sufficient to solve the equilibrium equation
M (Eq. 1.17)
1.3. Objectives and outline of the Thesis
The aim of this Thesis is the development of qualitative and quantitative studies of the local magnetic states of different ferromagnetic nanostructures such as Co and Co50Fe50 nanowires, Co antidot arrays and epitaxially strained La2/3Ca1/3MnO3 (LCMO)
thin films by in situ Lorentz Microscopy (LM) and Electron Holography (EH) experiments under the application of magnetic fields and working at low temperature
(100 K). For the development of in situ experiments with magnetic field, we have improved and generalized the traditional method where a controlled magnetic field is applied with the objective lens of the microscope, in a perpendicular direction of the sample plane. By a predictable double-tilt rotation of the sample, we have achieved a perfect control of the in-plane component of the magnetic field. Such magnetic field has been subsequently employed to perform magnetization reversal studies in different nanoscale ferromagnets, such as magnetic nanowires and antidot arrays. On the other hand, the use of a special TEM holder that cools down the sample to 100 K and reaches the ferromagnetic state of LCMO manganite has allowed us studying the effect of the substrate-induced strain in the magnetic properties of epitaxial LCMO manganite thin films.
This Thesis work has been structured in the present introduction (Chapter 1) followed by 6 chapters:
In Chapter 2 titled “Experimental Techniques”, we describe the main experimental techniques employed for the fabrication and characterization of the magnetic nanostructures investigated. Most of Chapter 2 is dedicated to a detailed description of the two main magnetic TEM characterization techniques: Lorentz microscopy and Electron Holography. In addition, we present the fundaments of the DualBeam Focus Ion/Electron Beam equipment, which is used to fabricate most of the nanostructures.
In Chapter 3 titled “In situ TEM characterization of magnetic nanostructures under external magnetic field”, we present the mathematical basis of the quantitative control of the in-plane magnetic field applied by the objective lens that allowed us improving the in situ LM and EH experiments. The validation of the calculation, as well as the effect of the unavoidable out-of-plane component of the magnetic field is evaluated through experimental measurements on different magnetic nanostructures grown by Focused Electron Beam Induced Deposition (FEBID). Finally, we show how local hysteresis loops can be reconstructed in magnetic nanostructures with high shape anisotropy with high accuracy, illustrating the method on a Fe-based Magnetic Tunnel Junction (MTJ) heterostructure.
Chapter 4 “Domain wall manipulation in Co and notched Co50Fe50 nanowires” is
devoted to the quantitative studies of domain wall (DW) manipulation in L-shape Co and (Co50Fe50) magnetic nanowires by in situ LM experiments. In the Co nanowires we
study the DW nucleation processes and the dependence of the DW nature with the nanowire lateral dimensions, while in the Co50Fe50 nanowires we evaluate the efficiency
of the field-driven propagation of DWs through sets of notches of different geometries.
In Chapter 5 titled “High-resolution imaging of remanent state and magnetization reversal processes in high-density cobalt antidot arrays”, we present the qualitative and quantitative studies of the remanent magnetic states of square cobalt antidot arrays of different periodicities. A high-density antidot array with a periodicity of 160 nm has been selected to study the magnetization reversal processes of this system through the nucleation and propagation of magnetic superdomains upon the application of a magnetic field along the easy and hard magnetization axes of the antidot array.
Chapter 6 titled “Strain-induced effects on the magnetic properties of epitaxial La2/3Ca1/3MnO3 thin films” explores the potential of low temperature EH experiments
by probing locally the changes in the magnetic configuration of strained LCMO thin films and the appearance of a non-ferromagnetic layer (NFL) at the surface. These experiments are combined with additional macro- and microscopic experimental techniques and first-principles calculations to understand the origin of this NFL.
Finally, in the Chapter 7, we summarize the main conclusions of this Thesis and draw new perspectives in this area.
 Lowther D A and Freeman E M 2008 The application of the research work of James Clerk Maxwell in electromagnetics to industrial frequency problems. Philos. Trans. A.
Math. Phys. Eng. Sci. 366 1807–20
 Terris B D, Thomson T and Hu G 2006 Patterned media for future magnetic data storage Microsyst. Technol. 13 189–96
 Wolf S A, Awschalom D D, Buhrman R A, Daughton J M, Von Molnár S, Roukes M L, Chtchelkanova A Y and Treger D M 2001 Spintronics: a spin-based electronics vision for the future. Science 294 1488–95
 Awschalom D and Samarth N 2009 Spintronics without magnetism Physics (College.
Park. Md). 2 50
 Picozzi S 2014 Ferroelectric Rashba semiconductors as a novel class of multifunctional materials Front. Phys. 2 1–5
 Uchida K, Takahashi S, Harii K, Ieda J, Koshibae W, Ando K, Maekawa S and Saitoh E 2008 Observation of the spin Seebeck effect. Nature 455 778–81
 Pauli W 1925 Über den Zusammenhang des Abschlusses der Elektronengruppen im Atom mit der Komplexstruktur der Spektren Zeitschrift für Phys. 31 765–83
 Hund F 1927 Linienspektren und Periodisches System der Elemente (Vienna: Springer Vienna)
 Stefanita C-G 2012 Magnetism (Berlin, Heidelberg: Springer Berlin Heidelberg)
 Heisenberg W 1928 Zur Theorie des Ferromagnetismus Zeitschrift für Phys. 49 619–36
 Weiss P 1907 L’hypothèse du champ moléculaire et la propriété ferromagnétique J.
Phys. Théorique Appliquée 6 661–90
 Kramers H A 1934 L’interaction Entre les Atomes Magnétogènes dans un Cristal Paramagnétique Physica 1 182–92
 Anderson P 1950 Antiferromagnetism. Theory of Superexchange Interaction Phys.
Rev. 79 350–6
 Ruderman M A and Kittel C 1954 Indirect Exchange Coupling of Nuclear Magnetic Moments by Conduction Electrons Phys. Rev. 96 99–102
 Kasuya T 1956 A Theory of Metallic Ferro- and Antiferromagnetism on Zener’s Model Prog. Theor. Phys. 16 45–57
 Yosida K 1957 Magnetic Properties of Cu-Mn Alloys Phys. Rev. 106 893–8
 Landau L and Lifshits E 1935 On the theory of the dispersion of magnetic permeability in ferromagnetic bodies Phys. Zeitsch. der Sow. 8 153–69
 Gilbert T L 1955 A Lagrangian formulation of the gyromagnetic equation of the magnetic field Phys. Rev. 100 1243
 Brown W F 1963 Micromagnetics (Michigan, USA: Interscience Publishers)
 Fischbacher T, Franchin M, Bordignon G and Fangohr H 2007 A Systematic Approach to Multiphysics Extensions of Finite-Element-Based Micromagnetic Simulations: Nmag IEEE Trans. Magn. 43 2896–8
 Vansteenkiste A, Leliaert J, Dvornik M, Helsen M, Garcia-Sanchez F and Van Waeyenberge B 2014 The design and verification of MuMax3 AIP Adv. 4 107133
 Abert C, Exl L, Bruckner F, Drews A and Suess D 2013 magnum.fe: A micromagnetic finite-element simulation code based on FEniCS J. Magn. Magn. Mater. 345 29–35
 Donahue M J and Porter D G 2012 OOMMF User’s Guide, Version 1.0, NISTIR 6376, National Institute of Standards and Technology
 Lopez-Diaz L, Aurelio D, Torres L, Martinez E, Hernandez-Lopez M A, Gomez J, Alejos O, Carpentieri M, Finocchio G and Consolo G 2012 Micromagnetic simulations using Graphics Processing Units J. Phys. D. Appl. Phys. 45 323001
2.1. TEM magnetic imaging 2.1.1. Introduction
The study of the magnetic properties of nanoscale ferromagnets requires the combination of macroscopic characterization techniques, which provide magnetic information averaged over large length scales, with local techniques capable of probing magnetic properties with high spatial resolution and sensitivity. Among the latter, magnetic imaging techniques permit a direct study of the magnetic configurations, particularly magnetic domain structures, at the submicron scale. The possibility of imaging ferromagnetic order, together with the improvement of the computational time of micromagnetic simulations, has significantly contributed to the understanding of the magnetic phenomena that has enabled the latest technological applications in the field of Nanomagnetism and Spintronics [1–3]. Today, there are a substantial number of magnetic imaging techniques. Among the most popular, we can list the Kerr microscopy based in the magneto-optical Kerr effect (MOKE); the scanning electron microscopy with polarization analysis (SEMPA); the spin-polarized low-energy electron microscopy (SPLEEM); synchrotron radiation-based techniques such as x-ray magnetic circular dichroism, photoelectron emission microscopy (XMCD-PEEM) and magnetic x-ray transmission microscopy (M-XTM); the scanning probe techniques such as magnetic force microscopy (MFM) and spin-polarized scanning tunneling microscopy (SP-STM); and TEM-based techniques such as Lorentz microscopy (LM) and electron holography (EH) [4–7]. All these experimental methods offer a wide range of possibilities to study micromagnetic phenomena in different setups, as can be seen in
the comparative list of their main features presented in Table 2.1. Altogether they provide a spatial resolution ranging from microns to few angstroms, time resolution down to nanoseconds, a high sensitivity to detect small changes of the local magnetization, probing the surface or the volume properties, and sufficient versatility to enable the application of multiple external stimuli (temperature, electromagnetic fields, etc.). None of these techniques covers all these possibilities, and they are therefore complementary.
Table 1.1.Summary of the main features of the most relevant magnetic imaging techniques
Technique Best spatial resolution Image acquisition time Type of imaging Type of depth information Information depth XMCD-PEEM 300 nm 0.03 - 10 s parallel surface < 5 nm Kerr Microscopy 200 nm 10-8 to 1 s parallel - scanning surface < 20 nm
MFM 40 nm 5 - 30 min scanning surface < 2 m
M-XTM 30 nm 3 s parallel - scanning
volume < 200 nm
SEMPA 20 nm 1 - 100 min scanning surface < 0.5 nm
SPLEEM 10 nm 1 s parallel surface < 1 nm
Lorentz Microscopy 10 nm 0.04 - 30 s parallel volume < 100 nm Electron Holography 1-2 nm 0.5 - 10 s parallel volume < 100 nm SP-STM lateral (0.2 Å); vertical (0.01 Å)
30 s – 30 min scanning surface < 0.2nm
From Table 2.1, we could classify the methods of magnetic imaging following different criteria that determines their range of application in terms of (spatial and time) resolution and sensitivity:
• The acquisition method: the image can be recorded using either a parallel acquisition of the signal in every point of the image simultaneously (e.g.
XMCD-PEEM, LM), or a serial acquisition in which a fine probe is scanned across the sample (e.g. MFM, SP-STM).
• The probe-specimen interaction on which the magnetic contrast is based: the Lorentz force experienced by electrons in the magnetic field of the sample (e.g. LM); the magnetic force on a magnetic tip caused by a stray field gradient (e.g. MFM); and magneto-optic coupling between photons and the magnetization of the material (e.g. Kerr microscopy); the Aharonov-Bohm effect in EH.
• The depth sensitivity, directly related to the probe-specimen interaction, determines whether the technique is sensitive only to the sample surface (e.g. MOKE, SPLEEM) or to the whole volume of the specimen such as in transmission techniques (e.g. M-XTM, LM and EH).
For the study of the local magnetic states, one of the most important requests is the achievable spatial resolution. This makes the TEM-based techniques very powerful tools that provide quantitative magnetic information of the volume of the sample with flexibility to apply external biases (magnetic and electric fields, injection of electrical current, changes in temperature, stress, light…) with a spatial resolution of few nanometers. The latter is only surpassed by SP-STM, whose spatial resolution goes down to atomic scale. To achieve the goals of the current “Nanotechnology revolution” – to understand and control matter at the nanoscale for industrial and technological application that benefit the society – magnetic TEM imaging techniques have become an indispensable instrument for the development of magnetic-based nanodevices.
Historically, the first attempts to study magnetic materials by TEM were to correlate the microstructure with the magnetic domain configuration measured by other techniques. For example, in 1958, Livingston explored the shape, size and distribution of ferromagnetic Co precipitates in relation with their magnetic characteristics [8,9]. A year before (1957), Mayer established the first method to observe the magnetism adapting an electron mirror microscope to observe artificial magnetic domain patterns produced by an array of linear magnetic stray fields and the magnetic contrasts of
ferromagnetic barium and nickel ferrite films . In 1959, M. E. Hale and collaborators developed the first methods to image domain patterns in ferromagnetic thin films through defocused TEM imaging  and, thanks to the use of an off-centered objective diaphragm, to image magnetic domains . These established the basis of LM in Fresnel and Foucault mode, respectively. In the 1970s and 1980s, other TEM-based magnetic techniques such as phase contrast microscopy [13–16] and off-axis EH (in the following, simply EH) [17,18] were developed. In these methods the magnetic information was obtained by retrieving the phase of the electron wave, although the electron beam phase shift measurements with sufficiently sensitivity had to wait for the development of high coherence electron sources which were available in commercial microscopes in the 90’s. The basic principle of EH is based on an original ideal proposed by Gabor , in 1949 to overcome the resolution-limiting spherical aberration of the objective lens. He proposed to perform an interferometric experiment in TEM by overlapping the exit electron wave that interacts with the object with an unperturbed electron wave that passes entirely through the vacuum (reference wave), allowing extracting the full information of the exit electron wave (amplitude and phase). Thus EH can be used to measure the phase shift of the electron wave that has interacted with a magnetic field and therefore to measure this magnetic induction (see section 2.3).
The most common magnetic TEM imaging techniques are LM in Fresnel mode and EH, which are the ones used in this Thesis. In the following, we will describe the image formation processes in TEM, showing how LM and EH solve one of the big challenges of TEM imaging: the retrieval of the phase shift of the electron wavefunction, which is usually lost in a conventional TEM imaging process.
2.1.2 Image formation in TEM
The overall process of the image formation in TEM can be summarized in six steps, which follow the electron wave trajectory:
1- Creation and acceleration of an electron beam from an electron source
3- Scattering of the electron wave by the specimen,
4- Formation of a diffraction pattern in the objective lens back focal plane,
5- Formation of an image of the specimen in the objective lens image plane.
6- Projection of the image (or the diffraction pattern) on the detector plane.
In the first step, electrons are generated either by thermoionic emission of a filament (tungsten or LaB6) heated at high temperatures, by the Cold Field Emission (C-FEG)
extraction from an extremely sharp tungsten tip (W(310)) at room temperature, or by the combination of both methods in a so-called Schottky Field Emission Gun (S-FEG). The C-FEG and S-FEG guns are highly coherent and bright electron sources, essential for EH and LM, while thermionic source provide more intense but poorly coherent beam. In the second step, the electron wave is accelerated (typically up to 60 kV to 300 kV) and the illumination system (a set of two or three condenser lenses) allows defining the beam (probe size, convergence angle, electron dose) that irradiates the top surface of the specimen. The electron wave then interacts with the sample through various processes of scattering, both elastic and inelastic. The exit electron wave coming out of the specimen is processed by the objective lens to form a diffraction pattern of the specimen in the back focal plane and subsequently an image of the object (Abbey’s theory of image formation in the microscope [20–22]). A schematic representation of the image formation in TEM following this simple idea is displayed in Figure 2.1(right-side).
The electron-specimen interaction makes that the incident electron wave changes its initial state by elastic and inelastic scattering phenomena. A summary of the signals generated in the electron-specimen interaction is also illustrated in Figure 2.1. In inelastic scattering processes, the electrons lose a small amount of energy that is transferred to the specimen producing the emission of a wide range of secondary signals (x-rays, visible light, secondary electrons, phonons and plasmons excitations), also damaging the specimen . These secondary signals are very useful to perform analytical TEM experiments such as x-ray energy-dispersive spectroscopy (XEDS),
electron energy-loss spectroscopy (EELS) or cathodoluminescence. On the other hand, in elastic processes the electrons are scattered without losing energy. In crystalline materials, the elastic scattering gives rise to Bragg diffraction related to the constructive interference of the scattered electron waves in a periodic crystal. Thus, Bragg scattering results in a series of diffracted beams scattered at angles dependent on the lattice periodicities of the crystal structure. The elastically scattered electron beams are the ones use to form images in TEM techniques such as diffraction-contrast TEM  and phase-contrast High Resolution TEM (HRTEM) .
Figure 2.1 (Left) Signals generated by the electron beam-specimen interaction. (Center) Basic schematic representation of the image formation by the objective lens in a TEM. Yellow lines represent the optical path followed by the electrons during the image formation process. (Right) The corresponding mathematical description of the image formation for an aberration-free TEM, where the information of the phase shift is loss.
The mathematical description of the image formation process in a TEM is described as follows. According to the quantum mechanics, the scattering of a high-energy electron plane wave interacting with a crystalline specimen can be well explained by the relativistic time-independent Schrödinger equation, also known as Dirac equation [26,27]. Considering a weak phase object approximation (electrons are scattered elastically by a thin specimen and absorption effects are neglected), its solution
Incident electron beam Direct electron beam Elastically scattered electrons Inelastically scattered electrons Bremsstrahlung X-rays Absorbed electrons Auger electrons Backscattered electrons Secundary electrons Characteris. X-ray Visible light SAMPLE ) (r obj ) ( ) (k Tk obj ) (r img 2 ) ( ) (r imgr I 2( ) r A )) ( exp( ) (r i r a )) ( exp( ) (r i r a Fourier transform Fourier transform T(k) = 0 For ideal microscope ) (r Sample Objective lens Back-focal planes Image planes